Paint Component Australia
Download Paint Component Australia...
NATIONAL ENVIRONMENTAL HEALTH FORUM
Paint Film Components
National Environmental Health Monographs General Series No. 2
Paint Film Components M van Alphen
National Environmental Health Forum Monographs General Series No. 2
National Environmental Health Forum
Paint Film Components
Copyright 1998 Copyright in this publication is assigned to the Department of Human Services on the basis of an agreement with M van Alphen Printed by Glenelg Press Published by the National Environmental Health Forum Prepared for publication by Bill Lock Public and Environmental Health Service Department of Human Services Price available on application. Correspondence with the author on Paint Film Components can be sent to: Mike van Alphen PO Box 3421 Rundle Mall SA 5000 Minor amendments have been made to page 8. The list of Published Monographs has been updated.
National Library of Australia Cataloguing-in-Publication; van Alphen, Mike. Paint film components. Bibliography. ISBN 0 642 30532 3. ISSN 1328 - 2867 1. Paint - Analysis. 2. Paint - Toxicology. I. National Environmental Health Forum. II. Title. (Series: National Environmental Health Forum Monographs. General Series; no. 2
Paint Film Components
Legislation affecting paint
1.2 Great Britain
1.3.1 Past legislation relating to paint manufacture and sale in Australia
1.3.4 New South Wales
1.3.5 South Australia
1.4 Occupational health and safety and paint in Australia 2.
The Paint Industry
2.1 The export and import of paints
2.2 The paint industry in Australia
2.3 Pigment manufacture
2.4 The early water paints - whitewash
2.5 Pigments and paint formulation practice
2.6 Pigment particle characteristics
2.7 After-treated and core pigments
2.8 World wide pigment utilisation
3.1 White lead
3.1.2 White lead manufacture processes
3.1.3 Properties of white lead
3.1.4 Imitation mother of pearl - white lead
3.2 White basic sulphate of lead
3.3 Red lead paint
3.4 Sublimed blue lead
3.5 Calcium plumbate
3.6 Lead titanate
3.7 Lead chlorides in paint
3.8 Lead chromates
The mixing of lead and zinc in paint
Zinc in paint
5.1 Zinc oxide
38 Paint Film Components
7.1.1 TiO2 from ilmenite
7.1.2 Anatase and rutile forms of TiO2
7.1.3 Trace components of titanium dioxide pigments
7.1.4 Extended TiO2
7.1.5 Was TiO2 a well known pigment in the 1940s?
Lead, Zinc Oxide, Lithopone and TiO2
8.1 TiO2 in Australia
8.2 Summary: TiO2 in paint
Other pigment materials
9.5 Cadmium pigments
9.6 Chromate pigments
9.6.2 Chrome green and fast chrome green
9.6.3 Chromium oxide
9.6.4 Zinc chromate
9.11 Mixed metal oxide pigments
9.12 Molybdate red and orange pigments
9.13 Organic pigments
9.14 Prussian blue: ferric ferrocyanide 9.14.1
10. Paint additives
10.2 Mineral whites, fillers or extenders
10.3.1 Asbestos, asbestine and other nomenclature
10.3.2 The function of asbestos in paint
Quantities of asbestos in paint Paint Film Components
The risk of asbestos in paint
Paint driers, old and recent
Driers: usual practice
The misuse of driers
10.5 Risks associated with paint driers
Surface disinfection in hospitals
10.7 Insecticidal paints
10.8 Mercury in paint
Mercury as a pigment
Substitutions for mercury as a pigment
Lingering use of mercury as a pigment
Mercury as a biocide
10.11 Thixotropic agents
11. Chlorine in paint
11.1 Chlorinated rubber
11.2 Polychlorinated biphenyls in paint
11.3 Chlorinated paraffins in paint
12. Metal primers: General
13. Metallic materials in paint
13.1 Metallic lead as a primer
13.2 Zinc dust metal paints
14. Luminous and fluorescent paints
15. Some non-household paints
15.1 Vehicle paints
15.2 Marine paints
16. Paint failure
16.1 Paint chalking descriptions
16.2 Paint chalking causes
16.3 Chalking of white lead paint
16.4 Susceptible pigments and modifications of pigments to address chalking
16.5 Properties of chalked paint surfaces
16.6 The risks of chalking paint
16.7 The durability and weathering of paint films
16.8 Gross failure
Alligatoring and cracking
17.1 Sandpaper abrasion of paint
96 Paint Film Components
17.2 Paint removal using heat
18. Paint solvents
19. Paint Substrates
19.2 Wood preservatives
19.4 Corrugated iron
19.5 Paint failure on cement
20. Lead in paint on Australian houses
20.2 Mort Bay, Sydney
20.3 Boolaroo, Newcastle
20.4 Port Pirie
20.5 Broken Hill
20.6 Paint lead in residential settings in Australia
20.7 Summary: The analysis of lead in paint in Australia
21. Paint covering and paint thickness, lead loadings and lead concentrations
21.1 Upper limits for lead content
21.2 Paint film thickness
21.3 Painted surface lead loadings
22. How much paint lead on a house?
23. The amount of lead in a chip of paint
24. Lead added to soils
Appendix 1 ~ Inorganic pigments
Appendix 2 ~ Paint pigments
Appendix 3 ~ Synthetic organic pigments
Paint Film Components
Acknowledgements My work in the South Australian Health Commission since 1993 has been directed towards the investigation of child lead exposure and lead smelter emissions with a limited emphasis on paint lead. An early draft of this work emerged after the realisation of the presence of paint film components such as asbestos, mercury, cadmium, and PCBs, among other components that may pose risks; in addition to those of lead. This project emerged (after hours) given the early encouragement of Mark Farfel, Rob Fowler and Nick Kim. For unpublished paint lead analysis data provided by Dani Boddington of the Broken Hill Environmental Lead Centre, and national paint lead survey data from Phil Anderson of the Australian Institute of Health and Welfare, I owe particular thanks. Two technical references provided a great deal of historical data for this work, the publishers of The Forensic Examination of Paints and Pigments (Charles C Thomas) and Paint Film Defects: their causes and cure (Chapman and Hall) have kindly provided permission to reproduce extended extracts from their works. Comments provided on the text by Andrew Langley and Nick Kim were very useful, the final preparation of the document, review of the text and checking of calculations by Bill Lock was readily appreciated. Any feedback on this work; be it requests for clarification, suggestions of alternate sources of information or any matters of debate; they would be greatly appreciated by the writer. Finally I thank Joe van Alphen - who has shared much practical knowledge, from some 40 years in the painting trade. Disclaimer This document has been prepared in good faith exercising due care and attention. However, no representation or warranty, expressed or implied, is made as to the relevance, accuracy, completeness or fitness for purpose of this document in respect of any particular user’s circumstances. Users of this document should satisfy themselves concerning its application to, and where necessary seek expert advice about, their situation. The NEHF, its participants and the SAHC shall not be liable to the purchaser or any other person or entity with respect to any liability, loss or damage caused or alleged to have been caused directly or indirectly by this publication.
Paint Film Components
Published monographs Water Series 1. Guidance for the control of Legionella (1996) 2. Guidance on water quality for heated spas (1996) 3. Guidance on the use of rainwater tanks (1998) Soil Series 1. Health-based soil investigation levels, 2nd edition (1998) 2. Exposure scenarios and exposure settings, 2nd edition (1998) 3. Composite sampling (1996) Metal Series 1. Aluminium, 2nd edition (1998) 2. Zinc (1997) 3. Copper (1997) Air Series 1. Ozone (1997) 2. Benzene (1997) 3. Nitrogen Dioxide (1997) 4. Sulfur dioxide (1999) General Series 1. Pesticide use in schools and school grounds (1997) 2. Paint film components (1998) 3. Guidelines for the control of public health pests – Lice, fleas, scabies, bird mites, bedbugs and ticks (1999) 4. National Standard for licensing pest management technicians (1999) Indigenous Environmental Health Series 1. Indigenous Environmental Health No. 1 (1999) Exposure Series 1. Child activity patterns for environmental exposure assessment in the home (1999) Counter Disaster series 1. Floods: An environmental health practitioner's emergency management guide (1999)
Paint Film Components
Preface This work provides an insight into the use of potentially toxic materials in paints, which may be left in the layers of paint films. The historical information presented is a guide to potentially toxic components in paint films and their probable concentrations. For example, it will permit a broad understanding of what paint components may be expected in a 100 year sequence of paint layers. Such a history is a preliminary step in the risk assessment process and will contribute to better informed decisions about the assessment and remediation of homes with old paints. Simply put, paint is a material that obscures and protects the underlying surface and is able to be pigmented with a range of colours. Paints by their protective functions, have to be environmentally stable, containing long lived materials that will form a waterproof barrier able to withstand biological, physical and chemical attack. The protective requirements of paints have commonly resulted in paint components being used which are potentially toxic as are some brilliantly coloured pigments. The manufacture of paints and pigments, particularly over the last hundred years, has been driven by the imagination and industry of millions of people and tens of thousands of manufacturing sites world wide. The diversity of raw materials and the different approaches to manufacture are responsible for wide variation in paint film composition. More subtle variations occur, particularly with respect to minor additives, whose concentrations may range over many orders of magnitude. Diversity in paint formulations is driven by the need for a range of colours, applied to a wide range of substrates, a diversity of paint uses and differing exposure (weathering) conditions. There are many paint properties such as covering or obscuring power, drying time, paint-film-hardness, film flexibility, colour permanence, water resistance, UV resistance, ease of application, control of paint layer thickness, rate of chalking, mould and fire resistance, among others, that are able to be modified by varying the properties and proportions of major components and minor additives. In many situations one component may require the addition of others to balance the physical and chemical properties of the formulation. The constitution of paint materials is highly varied as are the toxic properties of paint. Dusts generated by the abrasion of a number of different paint layers from a number of different surfaces of different ages may readily contain or be derived from several hundred different compounds. Some answers to questions on the contemporary risks related to old paint lie in the investigation of dried paint films. However, to estimate past exposures, particularly in relation to pesticides, organic mercury, and plasticisers which are sufficiently volatile for a proportion to be lost from the paint film over time, the analysis of original paint stored in good condition in-the-can may be useful. Such materials from the 1950s are rare but may still available from deceased estates or hazardous waste management depots, for example. The toxic properties of pigment particles or other materials in paint may be substantially influenced, and perhaps mediated, by the manner of encapsulation of that material by paint binding components. Examples of this may be the extent of encapsulation of asbestos fibres or lead-compound pigmentparticles by paint binders. The degree of rimming of potentially toxic particulates with paint binder and the nature of incorporation of toxic components with relatively inert components of a paint as well as their means of liberation from a paint film are central to detailed assessment of health risks. Since the 1950s, technology in pigment manufacture has resulted in pigment particles being individually encapsulated with layers often only nanometres thick of more stable compounds such as silicates. Any experimental, or occupational exposure based assessment of pigment toxicity, that has failed to characterise pigment particle coating, will also fail to represent the long term risk of highly weathered pigment where the pigment particle encapsulation has failed. Most animal studies of pigment toxicity fail to document the status of pigment particle coating. The 'quick and easy' assessment of the potential health risk of a particular component of paint films will be the total analysis. Matters which may mediate or accentuate risk such as the fate of inorganic and organic paint components; the sandwiching of toxic component rich paint layers among other Paint Film Components
paint layers, the bioavailability and particle size of toxic components at particular points in time, need to be considered when 'guideline' contaminant levels are being assessed. At various times, technical details relating to the manufacture of a pigment or the toxic properties of an ingredient may have been secret, poorly understood, or not considered to have been relevant to a particular manufacturing process and therefore not documented. Some details presented here may reflect the imperfect knowledge of the 1950s to 1970s. The use of potentially toxic paint components were frequently detailed in texts pre-1970, whereas such information appears to be rarely found post 1970. The chronology of discovery, use and withdrawal from use, of paint components is documented where possible, as is the history of legislation relating to paint. Legislated maximum levels of substances in paint in some situations, sometimes closely reflect actual levels and in numerous situations greatly exceed actual levels. In the 1950s and 1960s it was necessary for manufacturers, wholesalers and retailers, to hold more paint in stock than they do currently. In the past, in relation to already manufactured goods, legislation resulted in progressive declines in use of materials as stocks were cleared. Painting contractors and do-it-yourself painters may also store paints for future use. The date of enacting legislation may not mark the absence of future use of particular materials. In a small, isolated community, dominated by a single industry, it has been common for paints such as red lead and other industrial paints to have been widely used in the community. Aspects of past paint component use, particularly in the mixing of paint components by the user, involve modification of tradition, learned skills and behaviour. Such changes in behaviour are not implemented as rapidly or effectively as when all paint sold is ready to use. Ready-made paints gradually assumed dominance between the 1940s and late 1950s with the painting trade, but were more readily accepted by the do-ityourself painter, when they were available. The revolution in paint formulation in relation to lead risk was the reduction in use of white lead as the use of titanium dioxide pigments steadily increased, particularly from the early 1950s to the early 1960s. Over that period, Australia played a dominant role in the supply of titanium dioxide to world pigment markets. Titanium dioxide pigment, like other modern pigment particles, consists of a pigment core coated with a thin layer of material designed to improve the pigment characteristics. Detailed examination of titanium dioxide pigment shows that it has varied greatly over time in terms of its methods of manufacture and trace element chemistry. A summary of existing data on lead in paint on Australian houses provides useful insights as to what levels of lead in paint may be encountered. Models to evaluate the potential mass of lead on house walls are explored. Hundreds of kilograms of lead in paint are readily present on the walls of older houses. A 'typical' painting regime is outlined for a house built in 1900, having 280 m2 of wall area that resulted in a paint lead loading value of 103 mg Pb/cm2 such that the wall coatings would contain some 288 kg of lead. A worst case scenario indicated that some 364 to 644 kg of lead in paint on the walls is possible. Insights into the potential magnitude of soil contamination; given particular paint lead settings and scenarios for the incorporation of lead in soil, are readily obtained from models provided in this work. Even low levels of paint loss from an old wall surface will generate high soil lead concentrations. A 4m high wall having a paint lead loading of 80 mg Pb/cm2 which loses 10% of the lead from the wall will lose 320 grams of lead per linear metre of wall. If 85% of the lead lost from the wall is evenly incorporated into a 0.3m x 0.3m x 1.0m block of soil, the lead added to soil attributable to paint, would account for some 1780 mg of lead per kilogram of soil. A range of scenarios provide useful indications as to the likely ranges of concentration of soil lead attributable to paint lead. The substrate upon which a paint is applied should not be ignored when evaluating or testing paints for toxic components; lead may be encountered in plasters, putty and PVC. Timber treatment chemicals, and metal substrates, particularly plated metals may pose other problems. The tendency for particular paints to fail on particular substrates can help guide investigations into paint components. Paint Film Components
Much of the information on paint manufacture and formulation presented is generic. Most responses to, or comments on, health risks associated with paint will also be generic, based on common practice. However local paint manufacture or painting practice may result in more idiosyncratic use of paint components of which an investigator may need to be aware. Accounts of past formulation practice in the history presented here are not a complete assessment. Analysis of multi-layer paint films is one means of assessing matters such as the use and abundance of particular potentially toxic paint components suggested by the historical details of paint formulation. Paint solvents are discussed in this work, but are not investigated in detail. Paint is a universal component of the built environment and health risks associated with paints potentially impact on large numbers of people. Because of the long-lived nature of paint materials in residential settings, a good historical understanding of paint formulation and manufacture is required prior to undertaking scientifically valid health risk assessments.
Paint Film Components
Legislation affecting paint 1.1 International One of the early conventions directed towards the control of lead in paint was the International Labour Office (ILO) White Lead (Painting) Convention 1921 (No. 13) (Browne, 1983). According to Grut (1951) 27 countries had ratified the 1921 ILO convention which prohibited the use of white lead or sulphate of lead in 'internal' painting. The regulation of the use of toxic pigments and dye in the manufacture of edibles, foods and objects of daily use, in Germany, dates back to 1887, (Hess, 1965, p.205). Recent European regulations on cadmium use in pigments, are referred to in Buxbaum (1993, p.113114): 'In 1981 Sweden prohibited the use of cadmium pigments (with some exceptions) for ecological reasons. In 1987 Switzerland prohibited the use of cadmium pigments in plastics. Exceptions are possible if valid reasons can be given. In 1991 the EC passed a directive to prohibit the use of cadmium pigments as colorants for certain plastics that can be easily be coloured with other pigments. …. In 1996 the use in coating media will be prohibited. Use in artists' colors and ceramic products is still permitted.' And also from Buxbaum (1993, p.124): According to Directive EEC 89/178 (Feb 22 1989) and GefStoffV, ( April 23 1990), leadcontaining coatings and paints with a total lead content exceeding 0.15% of the total weight of the finished product must carry the warning: "Contains lead. Should not be used on surfaces liable to be chewed or sucked by children". A range of international, and national pigment manufacture standards and material specifications is listed in Buxbaum (1993, pp2-7). 1.2 Great Britain Similarities in legislation and standards between Australia and the UK were strong, particularly up to the 1970s. Regulations as to the methods of manufacture of lead pigments with regard to the control of occupational dust exposures appear to have been in place or introduced between the 1920s and 1940s (Hess, 1965, p.215). Early concerns were for the soluble lead content of paints ( Home Office Test for Soluble Lead S.R.&P., No. 1621, 1926).' The UK, Lead Paints (Protection against Poisoning) Act, 1926 restricted lead in paints as follows: For lead paints to be applied by spraying, the Act lays down a maximum figure (5 percent) for the lead compounds soluble in 0.25% hydrochloric acid, which is the concentration in normal digestive juices. This soluble-lead figure is calculated as lead monoxide (PbO) and is expressed as a percentage on the pigment. (see British Standard 282: 1963)[Morgans,1982, p.39] One interpretation of the above is that an extraction of a maximum of 5% lead, (calculated in terms of the PbO compound at 92.85% Pb) using a 0.25% HCl digestion of paint was permitted. This equates to paint returning an apparent analysis of 4.65 wt.% Pb by the weak HCl digestion method. According to Morgans (1982, p.39) in addition: Under the conditions of this method white lead and litharge are completely soluble, but the soluble lead contents of lead chromes and chrome greens vary according to the composition.
Paint Film Components
Morgans refers to the UK Lead Paint Regulations 1927 but does not report the details of this legislation. Hess (1965, p.212-213) notes various views on the restriction of paints for children's toys (BS 3443) as follows: 'the maximum of total toxic materials including lead has been restricted to 1 per cent on the dry film' and for other paints 'The British Paint Manufacturers' Executive Committee has recommended to its members that paints containing more than 1.5 per cent toxic materials on the dry film from January 1963 onwards should be labelled as unsuitable for surfaces likely to be chewed by children.' An article in October 1961 by Burgess, of London City Council is referred to in Hess (1965, p.66) as proposing '…limits for the amounts of toxic pigments contained in lacquers for children's crayons and pencils… In the lacquer for each pencil, etc., no more than 10 mgm. of metallic lead, soluble chromium, soluble barium, cadmium, selenium or acid soluble antimony or arsenic should be contained.' The above reference to metallic lead as opposed to soluble lead, may suggest some additional caution with respect to lead, Hess notes that the general proposal could be problematic if more than one toxic substance was present. The British Toys (Safety) Regulations, 1974 set a limit of 250 ppm "soluble" chromium in dry film, presumably to reduce risks in relation to the use of zinc chromates and CrVI , (Morgans, 1982, p.85). Many British Standards have in the past been considered de facto Australian Standards in the absence of local standards (Table 1). Building codes in the 1970s in various countries continued to require lead-based timber primers, by way of reference to standards despite lead reductions in paint. Table 1: Some British Standards from 1961 to 1976 (after Boxall and Frauhoffer, 1980) British Standard 217:
Red lead for paints and jointing compounds
British Standard 282:
Lead chromes and zinc chromes for paints.
British Standard 3698:
Calcium Plumbate Priming Paints
British Standard 3699:
Calcium Plumbate for Paints
British Standard 303:
Brunswick or lead chrome greens (pure and reduced) for paints.
British Standard 2523:
Lead-based Priming Paints
British Standard 239, 254, 1967: 338, 637 and 1851:
White pigments for paints
British Standard 4313:
Strontium chromate for paints
British Standard 318:
Chromic oxide pigments.
British Standard 3443:
Toy Paints: Code of Safety Requirements for Children's Toys and Playthings. (available prior to 1965 (Hess, 1965, pp.207).
British Standard 4310:
Permissible limit of lead in low-lead paints and similar materials
British Standard 5358:
Specification for low-lead solvent-thinned priming paint for woodwork.
1.3 Australia 1.3.1
Past legislation relating to paint manufacture and sale in Australia
The following section is a sample of the legislative regulations of paints. The history of legislative change is difficult to research and detailed understandings of the nature of implementation and outcomes of regulation will be difficult to evaluate. The following represents what was readily discovered in a limited time. Paint Film Components
A version of the Queensland Health Act (1937), of unknown age, which may or may not have been amended and then consolidated, and whose relationship with the Act of 1922 is unknown, is summarised here. The Queensland Health Act (1937) prohibited lead, arsenic or antimony in toys, wallpaper, decorative paper, paper serviettes and food wrapping paper amongst other things. In addition Section 127 restricted the soluble lead concentration of paints to 5% and prohibited the use of paints containing lead on roofs. It may well be that the Queensland legislation was very similar to the 1926 UK legislation. Section 127 of the Act did not appear to seek to legislate with respect to lead in interior paints. Structures already painted with 'soluble lead' could have attracted prosecution. Where paints in excess of 5% soluble lead were discovered, the State had the power to enforce the removal of that paint. Section 128 of the Act required the labelling of the name or names of ingredients and the quantity or percentage of each in the paint. It appears that this legislation was not designed to limit the amount of lead in paint (except roof paint) but to reduce the proportion of carbonate of lead to 5% (calculated as PbO), or 4.65 wt % lead soluble in weak hydrochloric acid. An undated pamphlet produced by the Australian Paint Manufacturers' Federation Inc., between 1993 and 1994, containing an endorsement from the Minister for the Environment, states: 'Prior to 1950 white lead was the principal white pigment used in house paints - although Queensland banned its use in 1922.' This assertion that white lead use was banned in 1922 has since been widely quoted, however the Queensland Health Act (1937) did not ban white lead; this did not happen until 1956. According to Hanson (1958), paints in Queensland up to that time were not lead free. More significant provisions relating to lead in paint became law in January 1956. The Struggle Against Lead Poison in the Painting Trade, Hanson (1958, p.7) makes the following comments regarding the 1956 law: 'The main points of the legislation are:(1) The manufacture, sale and use of paint containing basic lead carbonate (white lead) is banned in its entirety. (2) Paint containing lead of any description cannot be used on the roof of a house or other building or structure; any exterior portion of any house or other building whatsoever; any fence or gates whatsoever; any interior portion whatsoever of a house; or any household furniture. (3) Paint containing not more than 5% soluble lead chromate may be used on certain places but shall not be used on any exterior portion of a building which is accessible to children under fourteen years of age.' According to Hanson (1958, p.8) who quotes The Hon. WM Moore (ALP) from Hansard No 18, p.1295, 11/11/55: 'Our goal is now in sight. With the passing of the Bill to prevent the manufacture, sale and use of paint containing white lead, we can confidently look forward to the day when there will not be any white lead on any house in the State.' While Alperstein, Reznik and Duggin (1991, p.407) state that '....Australia led the world in measures to protect children from the hazards of lead poisoning when, in 1922, legislation was passed in Queensland banning the use of lead-based paint on verandahs and outside surfaces that were within the reach of children' the removal of white lead and reductions of lead in paint were a more drawn out process.
Paint Film Components
It appears that a 1942 Tasmanian Act relating to paint lead was based on the Queensland Act (pers. comm. Pamela Edwards, 1997). The Tasmanian Health Act 1962, sought to prohibit the sale, manufacture and use of paint containing basic carbonate of lead (Section 123), and sought to enforce restrictions and labelling requirements (Section 124) in relation to the total lead content of paints (Table 2). Table 2: Labelling requirements from the Tasmanian Health Act, 1962. Up to 1 % Pb
Containing not more than one percent of lead.
Between 1 and 5% Pb
Containing not more than five per cent of lead. For exterior use only -Not to be used on interior work or toys.
More than 5% Pb
Poisonous. Not to be used where food is or on roofs of buildings fences, or gates.
In addition, paints containing greater than 5% lead were prohibited from the exterior of a building (Section 125) although this was not obvious from the labelling requirements. Paints containing in excess of 1% lead were restricted from use in house interiors, on household furniture, and things that come in contact with food or water. Schedules were set for the allowable concentration of metals (Section 126) in or on toys, wall-paper, paper napkins or paper for enclosing food. Table 3: Class II classification by solvents and amount in the paint, relative to total (Tasmanian Statutory Rules, 1968) benzene
free organic isocyanates
The Tasmanian Public Health (Paint) Regulations 1968 designated a Class I paint as having Pb >1%, As >0.1%, Sb >5%, Cd >0.1%, Se >0.1%, Hg >0.5% of the non volatile content of the paint. Regulations required that percentages of all Pb, As, Sb, Cd, Se, or Hg be on a label of Class I paints. Such paints required warnings in relation to exposure of children to paint and were prohibited from: any toy, wallpaper, pencil, wrap, container, or furniture; the roof or other exterior portion of any house or other building or structure; any fence, wall, post or gate; any interior portion of any house or other building or structure intended for the use of human beings; or any household or other furniture or part thereof, [Tasmanian Statutory Rules, 1968] Class II paints were regulated in order to control solvent exposures to paint applicators, and risk of fire or explosion (Table 3).
Paint Film Components
New South Wales
Poisons Regulations under the Poisons Act 1966, contain provisions relating to the labelling of paints. Paints containing more than 1% Pb; 5% Sb; 0.1% As; 0.1% Cd; 5% chromate or dichromate; 0.1% Hg; 3% Sn; or 0.1% Se require the proportion of those compounds to be expressed, presumably on the label. Under 13A(5), ‘... In the case of a tinter containing 10 per cent or less of lead calculated as a proportion of the tinter, the proportion of lead contained therein may be omitted from the label.’ There was a NSW regulation from 14 January 1972 that incorporated a ban on paint lead carbonate (pers. comm., Edwards, 1997). Also, in relation to motor vehicle and industrial paints (Provision 13A(6)) a paint containing greater than 1% lead will not need to have the lead content printed on the label so long as 'FOR AUTOMOTIVE OR INDUSTRIAL USE ONLY' is written on the label. Industrial metal spray paints have been seen for sale in a hardware store in Broken Hill NSW, in late 1990 and, as recently as May 1995 similar paints in a range of bright colours with lead contents generally in the range 20-30%, have been seen in hardware stores in Port Pirie and Adelaide. The lead content of these paints is printed on the label. 1.3.5
It appears that in SA, until very recently, there has been no regulation of lead or other components in paint as it has been assumed that manufacturers have to conform with the regulations of others so as to trade interstate. In 1991 SA recognised the NHMRC Standard for the Uniform Scheduling of Drugs and Poisons (SUSDP) relating to paints. 1.3.6
The form of and date of commencement of any national Australian regulations or recommendations relating to paint standards from the 1960s is unknown. Anecdotal information suggests that such regulations existed. The NHMRC Standard for the Uniform Scheduling of Drugs and Poisons (SUSDP) had a standard that limited lead concentration in paint to 0.5% (in the non-volatile fraction of the paint) in 1990 which on 16 March 1992 was revised downward to 0.25% Pb (pers. comm. Keith McKellar). The use of lead and other chemicals in paints can restrict their use and impose labelling requirements (Table 4). The SUSDP limits the use of lead carbonate to mirror backings which in SUSDP, 1996 further specified no more than 15% Pb and application to less than 40 microns thickness. Table 4: Amounts of chemicals requiring labelling and use restrictions for paints (NHMRC, 1993, Appendix P) > 0.25% Pb or Pb compounds > 5% Sb or Sb compounds other than Sb titanate pigments > 5% Ba salts except BaSO4 or barium metaborate > 0.1% Cd or Cd compounds > 5% Cr as chromates of Ba, K, Na, Sr, Zn or NO3 > 0.1% Se or Se compounds
The manufacture, sale, supply or use of paints having concentrations of metals exceeding the levels in Table 4 is prohibited for the following applications: roofs or water collection surfaces; furniture; (and except on industrial sites) fences, walls, posts or gates, building interiors and exteriors (other than buildings solely for industrial purposes); and premises used for food processing.
Paint Film Components
The SUSDP in 1996, notes that after 1 December 1997 there will be additional labelling requirements for paints having greater than 0.1% Pb in the non-volatile fraction, lowering the previous level of 0.25% (NHMRC, 1996, p.249). In the case of zinc-based paints, additional labelling will be required when lead or lead compounds exceed 0.2%. From 1993, in relation to tinters containing more than 10% lead, the proportion of tinter required to raise the lead concentration of a paint above 2,500 ppm w/w is calculated and a warning is given to the effect that if greater than that certain amount of tinter is used then the use of the paint is to be restricted and labelled with additional warnings. A tinter containing more than 0.1% of lead is now to be labelled with the warnings: 'This tinter contains lead. Do not add to any paint which is for application to any toy, furniture, building (interior or exterior), fixed structure or to anything which may contact food or drinking water, and the expression KEEP OUT OF REACH OF CHILDREN. Table 5: Concentration of solvents in paints, above which labelling is required ([NHMRC, 1993, Appendix P). 1,2-Dichlorobenzene
5% by wt
5% by wt
5% by wt
Ethylene Glycol Monoalkyl Ethers
10% by vol
50% by vol
5% by wt
50% by vol
The SUSDP lists mercury in Schedule 7, where the warning DANGEROUS POISON is required on a label except where it is at or below 0.01 per cent organic mercury (100 mg/kg) as a preservative in paint (NHMRC, 1996, p.172). 1.4 Occupational health and safety and paint in Australia The Worksafe Australia standard for the 'Control of Inorganic Lead at Work' through the National Occupational Health and Safety Commission (NOHSC) has the objectives to: (a) minimise the risk of adverse health effects caused by lead exposure in the workplace by: (i) providing for assessment of the risk for jobs in the workplace where there is exposure, or potential exposure, to lead and to determine whether the job is a lead-risk job, (ii) ensuring that employees with potential exposure to lead used in a work activity are provided with information, induction and training on the nature of hazards and means of assessing and controlling exposure to workplace lead and that employee representatives have access to this information, (iii) ensuring that employers provide certain equipment and facilities, and provide for the testing and monitoring at workplaces where lead processes are conducted, and (iv) ensuring that emergency services and other relevant public authorities have access to relevant information on lead; (b) ensure that an employer controls lead exposure at the source in workplaces where lead processes are conducted; (c) ensure that an employer provides for the health surveillance of employees who work in leadrisk jobs; (d) prescribe certain duties of prescribed persons at workplaces where lead processes are conducted; Paint Film Components
(e) prohibit certain activities at workpIaces where lead processes are conducted; (f) ensure that information on lead exposures is available to public authorities (to be defined on a jurisdiction by jurisdiction basis); (g) ensure that this National Standard for the Control of Inorganic Lead at Work [ NOHSC: 1012(1994)] and National Code of Practice for the Control and Safe Use of Inorganic Lead at Work [ NOHSC:2015(1994)] are reviewed within four years; and (h) progressively reduce lead exposure and blood lead levels to convert existing lead-risk jobs to [NOHSC, 1994, pp.5-6] non-lead-risk jobs. The degree to which the Worksafe Australia Standard has been implemented with respect to the average painting contractor who would deal with lead-based-paints, particularly in respect of health surveillence is unknown. The definition of a lead risk job, means '...a work activity or a sequence of activities at specified workstations within the workplace, in which the blood lead level of the employee might reasionably be expected to rise, or does rise above 1.45 µmol/L (30µg/dl) or the removal level… whichever is the lower' (NOHSC, 1994, p.8). Where the worker is at or above the removal level, they are transferred from a lead-risk job to a non-lead-risk job. For males and females of non reproductive capacity the removal level is 50µg/dl, 20µg/dl for females of reproductive capacity, and 15µg/dl for pregnant or breast feeding females. (NOHSC, 1994, p.9 & 18). Based on sampling in the breathing zone, the lead in air exposure standard at October 1994, (the time weighted average concentration over a normal eight-hour working day) was 150 µg/m3, (NOHSC, 1994, p.13) whereas the Australian ambient lead in air NHMRC goal is 1.5µg of total suspended particulate lead per cubic metre of air (90 day average, 24 hour sample, 6 day cycle). There are two lead processes, defined in Schedule 1 of the Worksafe Standard that relate to paint: Machine sanding or buffing of surfaces coated with paint containing greater than one per cent by dry weight of lead. Any process whereby electric arc, oxy-acetylene, oxy-gas, plasma arc or a flame is applied, for the purpose of welding, cutting or cleaning, to the surface of any metal which is coated with [NOHSC, 1994, p.23] lead or paint containing greater than one per cent by dry weight of lead. In Schedule 2 (NOHSC, 1994, p.24) the following processes are relevant to paint: Spray painting with lead paint containing greater than one per cent by dry weight of lead. Working in any lead process not listed in Schedule 1 The above are defined as lead processes to which the national Worksafe Standard applies. Also in particular relevance to the painting trade, the Worksafe Standard prohibits among other techniques, the use of '…dry sweeping cleaning methods in lead process areas…' as well as the requirement to confine contamination by lead, as far as practicable, and ensure that lead contamination of the surrounding environment does not occur (NOHSC, 1994, p.13). Occupational health regulations in relation to solvents, 'nuisance dusts', and to some extent, heat-gun paint removal and chemical paint strippers have an impact on painting activities, but risks relating to paint components such as asbestos, mercury and other paint components for example are not explicitly recognised. A survey of 127 painters from North Carolina identified only three with blood lead levels between 20 and 30 mg/dl (Ennever, Zaccaro, Fernando, and Jones, 1995). According to a survey of home renovation in the year 1993-1994 in New York, some 86% of renovation was: '…conducted by persons who were not professional contractors and who may have been unaware of lead hazards and protective measures for safely containing dust and paint chips. Their work primarily involved sanding and scraping, methods that are potentially hazardous but require no training and little financial investment.' [quoting MMWR in JAMA, 1997, p.1031] Paint Film Components
The Paint Industry 2.1 The export and import of paints The Berger company claims to have been a major exporter to Australia prior to the 1900's but was not alone: 'Though Bergers were finding the competition tough in the domestic market, they were almost unopposed in their exports to the Colonies. A small but constant demand had been built up in the Australian colonies and almost every ship that left British ports for the months' - long trip [Cleary, circa.1956, p.23] to the young settlements carried stocks of Berger colours.' In 1907, one quarter of the British paint industry's product was being exported (Armitage, 1967, p.10). According to Cleary (c.1956, p.19) the Berger company based in North London in the early 1800's imported the raw materials for their paints, lead and quicksilver, from Spain. Such background information may be useful in relation to lead isotope analysis of paints to evaluate sources of child lead exposure. A prohibition on the export of white lead from the UK in WW1 appears to have been responsible for the beginning of the large scale manufacture of paint in Australia according to Technology in Australia 1788 - 1988 (Australian Academy of Technological Sciences and Engineering, 1988). 2.2 The paint industry in Australia An excellent compilation of the history of Australian Paint Manufacture is contained in Technology in Australia 1788-1988 (Australian Academy of Technological Sciences and Engineering, 1988). The following is a chronology, in most part, from that document: 1897
George Henry Taubman: importing painters supplies
George Henry Taubman: manufacturing paint at his Arncliffe home then at St Peters
The earliest recorded patent for a paint invention in Australia
Paint manufacture by H.L Vosz
Berger: had a warehouse in Sydney
Vosz formed the Australian United Paint Company (the first production site was in South Australia)
Wattyl paints started by the Walters family
Berger began to manufacture white lead in oil at Rhodes, (Homebush Bay) Sydney
British Australian Lead Manufacturers (BALM) formed from 3 Broken Hill mining companies and 7 white lead corroders, after the purchase of Australian United Paint Company
White lead exports from the UK were prohibited during WW1
BALM bought the Australasian United Paint Co of Port Adelaide (according to Rowe, 1983)
Prior to this time people generally made their own paints using imported pigments
Solver paint started around 1920 in Adelaide
BALM built a paint manufacture plant at Cabarita, Sydney
BALM had 26 lead stacks for the manufacture of white lead at Cabarita on the Parramatta River (Rowe, 1983)
Berger set up a factory in Wellington, New Zealand
Some time after 1924, ICI took a 40% interest in BALM
Around this time BALM and BHAS set up Commonwealth Litharge and Red Lead Pty Ltd. which appears to have been later bought by Dulux.
Australian Chemical Holdings/AC Hattrick imported phenol formaldehyde resins
Taubman had branches in 5 Australian states and NZ
Taubman became involved with USA paint producer Pinchin Johnson
Berger paint on the Sydney Harbour Bridge
First recorded manufacture of alkyds by BALM
Paint Film Components
Queensland Health Act (1937) restricted carbonate lead content of paint to 5% of total lead and prohibited the use of lead in paint on roofs
ICI began the local manufacture of nitrocellulose
Taubmans manufactured ethylenedichloride and DDT
BALM discovered a quick process for the manufacture of white lead that replaced the 3-4 month acetic acid and tanbark lead corrosion process
ICI obtained a 51% interest in BALM
Taubmans was Australia's 'second largest' paint company
ICI obtained a 70% interest in BALM
Wattyl became a public company, the third largest paint company in Australia (12% of market) Wattyl acquired Tafel-Shone, Usher, National Paints, Pioneer Chemicals, Kilrust, Davison and Spartan paint producers.
Tasmanian Health Act (1962) prohibition of carbonate of lead in paint and restricted the total lead content of exterior house paint to up to 5%
NSW Poisons Act (1966) paints containing > 1% Pb to be labelled.
Berger took over British Paints
Tasmanian Public Health (Paint) Regulations (1968) required the labelling of paints containing paints containing >1% lead.
Berger became a wholly owned subsidiary of Hoechst
BALM changed its name to Dulux Australia Limited
ICI obtained 100% ownership of BALM
Some technological milestones in industrial coatings with a focus on paint vehicles and paint systems, according to the Australian Oil and Colour Chemists Association (1983), include: 1915-20
Phenolic varnish resins
Low viscosity nitrocellulose Alkyd resins Anatase (TiO2)
Urea formaldehyde-alkyd blends Chlorinated rubber Molybdate orange pigments Vinyl chloride copolymers Phosphating and metal pretreatment
Phthalocyanine pigments Polyurethane resins Melamine formaldehyde-alkyd blends
Styrenated, acrylated oils Rutile (TiO2) Silicone Resins UV absorbers
Light fast organic yellows, oranges, reds, maroons, violets Unsaturated polyesters Polyamide cured epoxies Powder coatings
Acrylic automotive lacquers Thermosetting acrylic enamels Urethane oils Aqueous industrial primers Chloride process TiO2 Coal tar epoxy
Paint Film Components
Recent paint technology milestones according to Gooch (1993, pp.35-36), were focused more on the developments relating to paint vehicles: 1900s Kippling synthesized first polysiloxane. Rohm's PhD dissertation on polymerization of acrylic esters. 1901
Glyptal (thermosetting polyester) resins prepared by Smith from the condensation of glycerol and phthalic anhydride.
Baekeland produced first ethanol-soluble novalac; used as a substitute for shellac.
Amino-resins from urea and formaldehyde; patent application filed by John.
Soluble copolymers of vinyl chloride and vinyl acetate; patent applications filed by Reid of Union Carbide, and Voss and Dickahauer of IG Farbenindustrie.
Polyester resins improved by Kienle; applied unsuccessfully for patent for alkyd resins
Cellulose nitrate (trade name Duco) lacquers used in automobile finishes.
Alkyd name officially coined by Kienle for ester oils.
Oil-soluble varnishes patented by Turkington; produced by alkaline condensation with para-substituted phenols.
Glyptal and oleoresinous paint technology (oil-modified polyester resins) used by Kienle to produce superior polymers that were air-curable and more flexible than Glyptals; became known as alkyd resins.
Ethyl cellulose first went into commercial production.
Polyurethane resins originally synthesized by Bayer
Ethyoxyline resins patented by Schlack; became known as epoxy resins.
Polyvinylchloride plastisols were developed.
First styrene-butadiene latex commercialized for paper-coating application; first patents on pigmented paper coating issued in 1954 to S. D. Warren.
First styrene-butadiene latex sold for architectural-coating applications; prototype styrene-butadiene latex copolymer known as Dow latex 546.
Multicolored cellulose nitrates developed.
Powder coatings developed by Gemmer of Farbwereke Hoechst; granted a patent on the fluidized bed method of applying coatings using a powdered polymer. Ethyl acrylate and methyl methacrylate copolymer introduced as binders in house paints; the product was called Rhoplex# AC-33.
Cellulose acetate butyrate resin introduced for general purpose uses.
Acrylic esters replaced some cellulosic automobile coatings by General Motors.
Cellulose nitrate-isocyanate resins introduced. Alkyd-cellulose nitrate blends with copolymers of vinyl chloride and vinyl acetate used. Electrospray gun for applying powder coatings developed by Eraser and Point.
Cellulose nitrate lacquers ranked second among all industrial finishes.
Powder coatings used in Japan on automobiles and to a lesser degree in the United States; powder coatings eliminated volatile organic compounds.
1980s Powder coatings used extensively on appliances and automobiles as a substitute for enamels, thereby eliminating volatile organic compounds. 1990s Powder coatings expected to grow to 286 million pounds in North America and 507 million pounds annually in Europe.
Another chronology is available in Dick (1987, p.209).
Paint Film Components
2.3 Pigment manufacture Early pigment materials were raw minerals, ground and used on their own or mixed with other minerals. Simple processing such as calcining of pigments, reaction of metals to form oxides and carbonates, and the precipitation of pigment by reaction in solution may produce a range of compounds for use in paint formulation. While a manufacturing process may achieve a high efficiency in the conversion of material to a desired pigment phase, there is the potential for only 90 to 95% of the desired compound to be produced. For example, a range of lead carbonate mineral species might be encountered. Impurities in the raw materials or variations in process conditions may produce a range of different compounds (Table 6). Industrial quantities of pigment materials, particularly pre-1960 were of an industrial grade fit for a technical purpose and not single compound materials or 'chemically pure'. Pigment specifications and standards recognised this and often permitted the presence of a range of compounds. Table 6: Lead pigments, manufacturers and chemical compositions (Gooch, 1993, p196) Pigment
White lead pigment (circa 1950s)
Dutch Boy Co.
1. Pb3 (CO3)(OH)2 Lead carbonate hydroxide 2. PbCO3 Lead carbonate 3. Pb10(CO3)6(OH)6O Lead oxide carbonate hydroxide 4. Pb(BO2)2 ·H2O Lead metaborate hydrate
White lead pigment (circa 1950s)
1. Pb3 (CO3)2 (OH)2 / 95-97% Lead carbonate hydroxide 2. PbCO3 / 3-5% Lead carbonate
Red lead pigment (circa 1950s)
1. Pb3O4 Lead (II,III) oxide 2. Mg3SiO10 (OH)2 Talc mica (silicate)
White lead pigment (circa 1970s) Carter Chemical Co.
1. 3PbCO3·2Pb(OH)2 ·H2O Lead hydroxide carbonate hydrate
Red lead pigment
1. Pb3O4 Lead (II,III) oxide
Carter Chemical Co.
The commercial pressures to differentiate products in the marketplace, and the many possible routes to achieve similar bulk products will result in much variety in the mix of accessory compounds in pigment materials. Variations in the origin and amount of processing of mineral and chemical raw materials may also have a strong influence on accessory compounds in a bulk pigment product as well as an influence on trace elements in bulk pigment samples and trace elements within pigment particles. Accessory compounds such as lead acetate in the manufacture of white lead, may only have a small impact on the overall lead bioavailability of a particular paint sample, but the risk associated with accessory compounds cannot be overlooked. Particular methods for the precipitation of chromate pigment materials, for example, may increase the potential for the presence of hexavalent chromium or un-reacted hazardous starting or intermediate components in the final pigment. 2.4 The early water paints - whitewash Previous sections have listed the chronology of technological developments of paint materials from a range of perspectives. One aspect of paints that is poorly documented in the literature appears to be that of essentially chalk and glue - water based paints and similar lime based paints. They have been unchanged in their essential characteristics for a long time. They are cheap materials and as all the ingredients are readily available, perhaps not seen as a major concern of those in mainstream commercial ready-made-paint manufacture.
Paint Film Components
Water paints were common pre-1960; they cannot be readily compared with what we know of oil and present water-based paints. They were commonly purchased as dry powder in a cardboard carton. The cheapest of these paints when used outdoors have to be regularly applied owing to the high rate of erosion of the paint surface. In some settings where 'water paints' are widely used, the concept of paint layers accumulating in thickness with each generation of painting, to make multi-layer paint films, may not be relevant. In such settings the rate of addition of paint components to soil may be elevated with respect to modern water-based and enamel paints. Calsimine (also Kalsomine) made by the painter is based on whiting, (chalk, CaCO3) and may also contain glue size, pigments for tinting, and water (Holloway, 1953, Vol.I, p.183). The problems associated with glue and for example casein in paint is that these components may sustain mould growth and there is a need for additives to combat this problem before and after application. Distempers contain glue (DLNS, 1955) and are probably similar to calsimine. Emulsion paints include components that don't normally mix and could be oil-in-water (or water-inoil) emulsions and for example may contain, linseed oil, casein, water and pigment (DLNS, 1955, p.36). Limewash, is essentially a lime-based thin cement wash, which may contain many of the components of emulsion or water paints and is not able to be painted-over by oil or water paints. It is difficult to remove and for that reason is a troublesome material to use (Holloway, 1953, Vol.I, pp.195-197). Holloway (1953, Vol. I, p.192) distinguishes between the ordinary calsimine and the washable water paint. The washable material is not so readily removed, and the adhesion may be highly variable. Washable waterpaint poses greater risk of failure by cracking or peeling, as it has relatively poor surface adhesion properties causing problems particularly when additional coats of washable water paint are added on top of this or other material, and its use is associated with '…some danger of premature failure' (Holloway,1953, Vol. I, p.193). Table 7: Pigments compatible with lime or chalk-based waterpaint (Holloway, 1953, Vol.I, p.185). Sienna, raw and burnt
Umber, raw and burnt
All the black pigments
White lead or lead chromate pigments are not likely to have been used in lime-based or chalk-based waterpaint but Table 7 lists some compatible pigments. A later section on paint substrates lists a similar array of pigments that are compatible with cement, lime and plaster. An early form of plastic paint was available in dry powder or paste form and thinned with water (Holloway, 1953, Vol. II, p.138) and used for thick, textured effects on surfaces. Such early waterbased paints may not have been chalk-based. The textured plastic paints appear to have been the forerunners of water-based plastic, chlorinated rubber, PVC, PVA and latex paints which began to replace oil based paints for interior surfaces in the 1960s.
Paint Film Components
2.5 Pigments and paint formulation practice Developing technology and the availability of new raw materials has had major impacts on paint formulation over time. Atlas Chemical Company, Sunderland (1896, p.1) recommended for some pigments the calcining of rough ground mineral ores in a crucible, this mixture was then finely ground. Elsewhere (p.130) fine pigment powder was to pass a sieve containing 80 holes to the inch. Such was the simplicity of early processes. The paint recipes from Atlas Chemical Company (1896) contain a greater number of formulations utilising bichromate of potash, antimony, chromium oxide, copper oxide and tin oxide than is seen in recipes from about the 1920s onward. This may reflect the more general practice at that time. According to Cleary (c.1956, p.29), around 1911 in Australia, when the Berger company was operating a depot in Sydney ' White lead and linseed oil were the accepted bases with tradesmen painters; prepared paint was something only amateur painters indulged in'. In Australia prior to 1920 painters would mostly have mixed their own paints using imported pigments, due to the absence of local manufacture. According to Jennings (1926, p.191) by 1926 the grinding of dry pigment in oils '...is carried on by most of the large manufacturing paint houses, many of whom do not themselves make the dry pigments.' Vanderwalker (1944, p.76), notes that: 'At some time or other most painters and decorators wonder why they cannot make their own ready-mixed or prepared paints and save some money. They learn that formulas for these materials contain such inert materials as silica, barytes, whiting, asbestine or magnesium silicate; they note that prices on inert pigments are much less than for white lead and zinc, and wonder why they cannot make cheaper paints than they can buy from manufacturers.' The author then begins to make a case for the complexity of paint formulation. It appears that the period from the 1920s to the 1950s is one of major transition from paints primarily mixed on site with raw ingredients to paints primarily purchased in a more ready-made condition. While early use of white lead was as dry powder, in the 1950s white lead was available as a paste, said to be '...marketed in three different consistencies-stiff, medium, and soft-to meet varying requirements,…' Holloway, (1953, Vol.I, p.208). Vanderwalker (1944, p.69) was still able to secure white lead as a dry powder, but: '...it is more commonly used as a thick paste which is composed of 92 per cent white lead and 8 per cent linseed oil. Most of the white lead now sold to painters is in soft paste form (also called all-purpose white lead), which is much easier to mix than the older heavy paste lead. Soft paste contains approximately 85 per cent white lead and 15 per cent liquids - linseed oil and turpentine.' Basic lead carbonate pigment mixed with linseed oil and turpentine into a painting consistency and left to stand for some days, will be too thick, even after stirring, and will require the addition of more oil (Vanderwalker, 1944, p. 123). Manufacturers of prepared paints were often just mixers and formulators of paints, dealing in a market with thousands of potential ingredients. Armitage (1967 p.105) considered that a large proportion of paint formulation work was '...concerned with the examination of new products from raw material suppliers, which are offered in embarrassingly increasing quantities.' A useful list of colours associated with metal pigments is given in Crown (1968) in The Forensic Examination of Paints and Pigments, the next most comprehensive and historically useful listing may be Jennings (1926) Paint and Colour Mixing , and Vanderwalker (1944) The Mixing of Colours and Paints, some of which are reproduced in Appendices to this document. Paint Film Components
Turczynowicz (1991, p.50 ), Burgess (1981, p.103) and Morgans (1982, p.282) give similar listings of pigments. Armitage (1967, p.116) states that 'Modern enamels usually have no extender, and relatively poor hiding power, the amount of titanium dioxide present being about 60-70% of the weight of solid binder.' Such views indicate a lack of acceptance of 'modern' TiO2 paints. Table 8: Typical pigment levels in liquid paints (Boxall and von Frauhoffer (1980, p.38) White
Basic lead silichromate
Basic lead sulphate
Lead chrome green
Black iron oxide
Yellow Lead chromates
The critical pigment volume concentration is discussed by Patton (1964, pp.186-187). It is a point of compromise between a high gloss, low permeability paint susceptible to blistering and a permeable flat paint with insufficient connectivity of pigment by the binder component to protect the substrate from rusting or other decay. Levels of pigment in liquid paint are usually 10 to 30% (v/v) but can be as low as 1% and as high as 70%. 2.6 Pigment particle characteristics The mean particle sizes of inorganic pigments according to Buxbaum (1993, p.14) '...lie in the range 0.01 - 10 µm, and are usually between 0.1 and 1µm.' By another generalised account, paints can contain 20-60% by weight of pigment generally ground to less than 3 microns ranging from 0.5 to 10 microns (IARC, 1989). Buxbaum (1993, p.24-25) notes how Mie's Theory predicts a maximum in light scattering at an optimal particle diameter, where for example titanium dioxide creates optimal scattering (550 nm wavelength) at some 0.2 ± 0.1 microns. This calculated scattering by titanium dioxide is some 3 times greater than that of zinc oxide and white lead which produce maximum scattering at some 0.5 ± 0.3 microns particle diameter. Such optimal pigment particle sizes are likely to be targeted during pigment manufacture. TiO2 pigment particles with a size less than or equal to '...0.2 µm scatter light of shorter wavelengths more strongly and therefore show a blue tinge, while larger particles have a yellow tone.' (Buxbaum, 1993, p.66).
Paint Film Components
Paint pigment particle morphology will be dependent on the crystallographic form of the pigment compound, and the degree of modification due to grinding or precipitation on the pigment particle surface. An advance in the grinding and dispersion of pigments in the early 1950s is attributed to the sand or bead mill, (Armitage 1967, p.96 & p.99) developed by Du Pont. Buxbaum (1993, p.98) refers to jet milling (micronisation) as a particle size reduction method. In the examination of sequences of paint layers it is common to see more coarse pigment and filler particles for example in the range from 5 to 15 microns in older layers and in priming and undercoat layers. Asbestos was added to the paint to exploit the properties of its long, slender fibres. Hess (1965, p.136) notes surface imperfections of 0.5mm can affect gloss and that while aggregates, agglomerates or flocculates of pigment can affect gloss, an effective means of obtaining flattness of finish is to employ relatively coarse inert particles. While the possibility of pigment agglomeration as a consequence of paint formulation (Hess, 1965, p.88) has been raised, and the potential for agglomerates at 1 to 100Τm (p.136) noted, the prevalence of this phenomenon is unknown. Further, the degree to which most painters would routinely strain paint through stockings or sieves (Brindley, ca.1952, p.20) to remove 'pips' from new and 'used' paint is unknown. This is a matter of workmanship which in the past was an important step in order to obtain smooth glossy top coats. The use of mixtures of pigment of differing morphology in the one formulation has appeared to have been a strategy employed in the past: ‘The shape of the ground-in pigments may also exert a certain influence, i.e. spherical-shaped pigments such as zinc oxide and splinter-shaped particles of barium sulphate if mixed together yield a much denser and more protective texture than if used unmixed. (M. Ragg.) The same applies to needle-shaped structures due to their felting tendencies (Depew) as long as they are [Hess, 1965, p.292] not ground too finely or if they are very hard.’ Gloss paints and automotive paints are likely to have very finely ground pigment particles relative to, for example, flat paints, fire resistant paints and paints for concrete and masonry (Patton, 1964, pp. 208-209). The distribution of lead in sandblasting residue, which includes the spent blasting abrasive, is such that no fine or coarse fractionation of lead occurs; it is distributed somewhat evenly across sieve sizes from